#------------------------------------------------------------------------------
#$Date: 2016-03-25 11:21:14 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179786 $
#$URL: svn://www.crystallography.net/cod/cif/7/00/82/7008267.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7008267
loop_
_publ_author_name
'Copping, Roy'
'Gaunt, Andrew J.'
'May, Iain'
'Sarsfield, Mark J.'
'Collison, David'
'Helliwell, Madeleine'
'Denniss, Iain S.'
'Apperley, David C.'
_publ_section_title
;
 Trivalent lanthanide lacunary phosphomolybdate complexes: a structural
 and spectroscopic study across the series [Ln(PMo11O39)2]11-.
;
_journal_issue                   7
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1256
_journal_page_last               1262
_journal_paper_doi               10.1039/b500408j
_journal_year                    2005
_chemical_formula_sum            'H78 La Mo22 N11 O95 P2'
_chemical_formula_weight         4064.26
_chemical_name_systematic
;
?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 118.033(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   37.866(5)
_cell_length_b                   13.0069(16)
_cell_length_c                   19.640(2)
_cell_measurement_reflns_used    7799
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      28.3415
_cell_measurement_theta_min      2.2705
_cell_volume                     8538.2(18)
_computing_cell_refinement       'SAINT, Bruker'
_computing_data_collection       'SMART, Bruker'
_computing_data_reduction        'SAINT, Bruker'
_computing_molecular_graphics    'XSHELL, Bruker'
_computing_publication_material  'XP, Bruker; Diamond 2.1e, Crystal Impact'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.930
_diffrn_measured_fraction_theta_max 0.930
_diffrn_measurement_device_type  'SMART platform CCD, Bruker'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0192
_diffrn_reflns_av_sigmaI/netI    0.0210
_diffrn_reflns_limit_h_max       49
_diffrn_reflns_limit_h_min       -48
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            29659
_diffrn_reflns_theta_full        28.34
_diffrn_reflns_theta_max         28.34
_diffrn_reflns_theta_min         1.68
_exptl_absorpt_coefficient_mu    3.775
_exptl_absorpt_correction_T_max  0.6601
_exptl_absorpt_correction_T_min  0.3972
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS, Bruker'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.162
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             7704
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.12
_refine_diff_density_max         2.431
_refine_diff_density_min         -1.206
_refine_diff_density_rms         0.285
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.311
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     529
_refine_ls_number_reflns         9920
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      1.311
_refine_ls_R_factor_all          0.0463
_refine_ls_R_factor_gt           0.0455
_refine_ls_shift/su_max          0.009
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+546.3666P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1159
_refine_ls_wR_factor_ref         0.1163
_reflns_number_gt                9777
_reflns_number_total             9920
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b500408j.txt
_cod_data_source_block           ajg43c2c
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               7008267
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
La1 La 0.0000 0.84726(5) 0.2500 0.00807(13) Uani 1 2 d S . .
Mo7 Mo 0.10896(2) 0.60030(6) 0.09531(4) 0.00954(14) Uani 1 1 d . . .
Mo1 Mo 0.10970(2) 0.95577(6) 0.37244(4) 0.00770(14) Uani 1 1 d . . .
Mo4 Mo 0.02214(2) 0.66237(6) 0.10567(4) 0.00844(14) Uani 1 1 d . . .
Mo6 Mo 0.06626(2) 0.83675(5) 0.03808(4) 0.00861(14) Uani 1 1 d . . .
Mo2 Mo 0.06472(2) 1.02085(5) 0.18610(4) 0.00752(14) Uani 1 1 d . . .
Mo9 Mo 0.15997(2) 0.96721(5) 0.17452(4) 0.00813(14) Uani 1 1 d . . .
Mo5 Mo 0.15926(2) 0.69994(6) 0.43218(4) 0.00973(14) Uani 1 1 d . . .
Mo8 Mo 0.16002(2) 0.52789(5) 0.30254(4) 0.00840(14) Uani 1 1 d . . .
Mo10 Mo 0.20513(2) 0.89305(6) 0.36290(4) 0.00912(14) Uani 1 1 d . . .
Mo11 Mo 0.20429(2) 0.73108(6) 0.22579(4) 0.00881(14) Uani 1 1 d . . .
Mo3 Mo 0.07138(2) 0.58679(6) 0.30594(4) 0.00926(14) Uani 1 1 d . . .
N1 N 0.2314(3) 0.1016(7) 0.0705(5) 0.0244(18) Uiso 1 1 d . . .
N2 N 0.1611(3) 0.2273(7) 0.5042(5) 0.0217(17) Uiso 1 1 d . . .
N3 N 0.0317(3) 0.7816(7) 0.8246(5) 0.0199(17) Uiso 1 1 d . . .
N4 N 0.1532(3) 0.2053(7) 0.2892(5) 0.0240(18) Uiso 1 1 d . . .
N5 N 0.0695(3) 0.3584(7) 0.1475(5) 0.0217(17) Uiso 1 1 d . . .
N6S N 0.2323(15) 0.1024(16) 0.585(3) 0.047(11) Uiso 0.25 1 d P . .
N6T N 0.2334(12) 0.167(3) 0.456(2) 0.029(8) Uiso 0.25 1 d P . .
O1 O 0.06181(17) 0.9224(5) 0.3577(3) 0.0104(11) Uani 1 1 d . . .
O2 O 0.02169(17) 0.9883(5) 0.1923(3) 0.0098(11) Uani 1 1 d . . .
O3 O 0.04724(18) 0.7014(5) 0.3011(3) 0.0110(12) Uani 1 1 d . . .
O4 O 0.00986(18) 0.7648(5) 0.1480(3) 0.0104(11) Uani 1 1 d . . .
O5 O 0.12840(19) 1.0280(5) 0.4536(4) 0.0141(12) Uani 1 1 d . . .
O6 O 0.09514(17) 1.0560(4) 0.2956(3) 0.0084(11) Uani 1 1 d . . .
O7 O 0.05516(18) 1.1422(5) 0.1490(4) 0.0123(12) Uani 1 1 d . . .
O8 O 0.13135(17) 0.8192(5) 0.4185(3) 0.0102(11) Uani 1 1 d . . .
O9 O 0.09144(16) 0.8666(4) 0.2550(3) 0.0065(10) Uani 1 1 d U . .
O10 O 0.11456(18) 0.6129(5) 0.4090(3) 0.0110(12) Uani 1 1 d . . .
O11 O 0.05671(17) 0.9447(5) 0.0991(3) 0.0090(11) Uani 1 1 d . . .
O12 O 0.04470(19) 0.4959(5) 0.3236(4) 0.0157(13) Uani 1 1 d . . .
O13 O -0.02211(18) 0.6031(5) 0.0503(4) 0.0147(13) Uani 1 1 d . . .
O14 O 0.04662(18) 0.5798(5) 0.1929(3) 0.0111(12) Uani 1 1 d . . .
O15 O 0.02133(18) 0.7663(5) 0.0265(3) 0.0105(11) Uani 1 1 d . . .
O16 O 0.05464(17) 0.5834(5) 0.0635(3) 0.0119(12) Uani 1 1 d . . .
O17 O 0.04840(18) 0.9020(5) -0.0465(3) 0.0112(12) Uani 1 1 d . . .
O18 O 0.11214(18) 0.4884(5) 0.3000(3) 0.0111(12) Uani 1 1 d . . .
O19 O 0.08839(17) 0.7402(4) 0.1547(3) 0.0071(11) Uani 1 1 d . . .
O20 O 0.12198(17) 0.6895(4) 0.2933(3) 0.0069(11) Uani 1 1 d . . .
O21 O 0.12458(17) 1.0273(5) 0.1976(3) 0.0096(11) Uani 1 1 d . . .
O22 O 0.18358(18) 0.6882(5) 0.5289(3) 0.0134(12) Uani 1 1 d . . .
O23 O 0.16447(17) 0.9538(5) 0.3698(3) 0.0095(11) Uani 1 1 d . . .
O24 O 0.24639(18) 0.9420(5) 0.4382(3) 0.0148(13) Uani 1 1 d . . .
O25 O 0.20271(17) 0.9780(5) 0.2818(3) 0.0100(11) Uani 1 1 d . . .
O26 O 0.19759(17) 0.7722(5) 0.4142(3) 0.0097(11) Uani 1 1 d . . .
O27 O 0.15394(17) 0.8210(5) 0.2468(3) 0.0089(11) Uani 1 1 d . . .
O28 O 0.18084(17) 0.5755(5) 0.4023(3) 0.0110(12) Uani 1 1 d . . .
O29 O 0.12099(17) 0.8970(5) 0.0920(3) 0.0105(11) Uani 1 1 d . . .
O30 O 0.12620(18) 0.5297(5) 0.1849(3) 0.0115(12) Uani 1 1 d . . .
O31 O 0.08919(17) 0.7233(5) 0.0201(3) 0.0104(11) Uani 1 1 d . . .
O32 O 0.11572(19) 0.5165(5) 0.0362(4) 0.0158(13) Uani 1 1 d . . .
O33 O 0.18377(18) 0.4143(5) 0.3134(4) 0.0143(12) Uani 1 1 d . . .
O34 O 0.15767(17) 0.6758(5) 0.1386(3) 0.0110(12) Uani 1 1 d . . .
O35 O 0.19280(18) 0.6149(5) 0.2788(3) 0.0113(12) Uani 1 1 d . . .
O36 O 0.19755(17) 0.8539(5) 0.1749(3) 0.0098(11) Uani 1 1 d . . .
O37 O 0.17537(18) 1.0613(5) 0.1344(4) 0.0122(12) Uani 1 1 d . . .
O38 O 0.23116(17) 0.7908(5) 0.3227(3) 0.0103(11) Uani 1 1 d . . .
O39 O 0.24189(19) 0.6748(5) 0.2152(4) 0.0148(13) Uani 1 1 d . . .
O1S O 0.2127(2) 0.4604(6) 0.1815(5) 0.0286(17) Uiso 1 1 d . . .
O2S O 0.1854(2) 0.5601(6) 0.0294(5) 0.0291(17) Uiso 1 1 d . . .
O3S O 0.1721(2) 0.2748(6) 0.1740(4) 0.0264(16) Uiso 1 1 d . . .
O4S O 0.2307(3) 0.1971(7) 0.3977(5) 0.0182(18) Uiso 0.75 1 d P . .
O5S O 0.1066(2) 0.2873(6) 0.3476(4) 0.0267(16) Uiso 1 1 d . . .
O6S O 0.0112(2) 0.3816(6) 0.3969(5) 0.0301(17) Uiso 1 1 d . . .
O7S O 0.9511(2) 0.8819(7) 0.0090(5) 0.0311(18) Uiso 1 1 d . . .
O8S O 0.9015(3) 0.7056(7) 0.9561(5) 0.0341(19) Uiso 1 1 d . . .
O9S O 0.2332(3) 0.1131(7) 0.5299(5) 0.0185(18) Uiso 0.75 1 d P . .
P1 P 0.11349(6) 0.78045(16) 0.23761(12) 0.0066(4) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 La1 O4 128.1(3) . 2 ?
O4 La1 O3 72.0(2) . 2 ?
O4 La1 O3 68.7(2) 2 2 ?
O4 La1 O3 68.7(2) . . ?
O4 La1 O3 72.0(2) 2 . ?
O3 La1 O3 79.8(3) 2 . ?
O4 La1 O2 75.0(2) . . ?
O4 La1 O2 154.7(2) 2 . ?
O3 La1 O2 135.30(19) 2 . ?
O3 La1 O2 114.8(2) . . ?
O4 La1 O2 154.7(2) . 2 ?
O4 La1 O2 75.0(2) 2 2 ?
O3 La1 O2 114.8(2) 2 2 ?
O3 La1 O2 135.30(19) . 2 ?
O2 La1 O2 85.1(3) . 2 ?
O4 La1 O1 114.89(19) . . ?
O4 La1 O1 85.5(2) 2 . ?
O3 La1 O1 148.6(2) 2 . ?
O3 La1 O1 75.3(2) . . ?
O2 La1 O1 73.70(19) . . ?
O2 La1 O1 72.85(19) 2 . ?
O4 La1 O1 85.5(2) . 2 ?
O4 La1 O1 114.9(2) 2 2 ?
O3 La1 O1 75.3(2) 2 2 ?
O3 La1 O1 148.6(2) . 2 ?
O2 La1 O1 72.85(19) . 2 ?
O2 La1 O1 73.69(19) 2 2 ?
O1 La1 O1 134.0(3) . 2 ?
O32 Mo7 O30 103.7(3) . . ?
O32 Mo7 O16 101.1(3) . . ?
O30 Mo7 O16 95.9(3) . . ?
O32 Mo7 O34 102.2(3) . . ?
O30 Mo7 O34 89.8(3) . . ?
O16 Mo7 O34 153.9(3) . . ?
O32 Mo7 O31 97.4(3) . . ?
O30 Mo7 O31 158.6(3) . . ?
O16 Mo7 O31 83.1(3) . . ?
O34 Mo7 O31 82.5(2) . . ?
O32 Mo7 O19 167.5(3) . . ?
O30 Mo7 O19 87.9(2) . . ?
O16 Mo7 O19 72.7(2) . . ?
O34 Mo7 O19 82.2(2) . . ?
O31 Mo7 O19 71.3(2) . . ?
O5 Mo1 O1 103.6(3) . . ?
O5 Mo1 O6 101.9(3) . . ?
O1 Mo1 O6 98.6(3) . . ?
O5 Mo1 O8 99.6(3) . . ?
O1 Mo1 O8 91.5(3) . . ?
O6 Mo1 O8 153.2(2) . . ?
O5 Mo1 O23 92.9(3) . . ?
O1 Mo1 O23 162.0(3) . . ?
O6 Mo1 O23 84.8(2) . . ?
O8 Mo1 O23 78.4(2) . . ?
O5 Mo1 O9 170.9(3) . . ?
O1 Mo1 O9 85.0(2) . . ?
O6 Mo1 O9 73.5(2) . . ?
O8 Mo1 O9 82.9(2) . . ?
O23 Mo1 O9 79.0(2) . . ?
O13 Mo4 O4 104.4(3) . . ?
O13 Mo4 O14 104.0(3) . . ?
O4 Mo4 O14 97.6(3) . . ?
O13 Mo4 O15 99.0(3) . . ?
O4 Mo4 O15 86.9(3) . . ?
O14 Mo4 O15 154.6(3) . . ?
O13 Mo4 O16 96.5(3) . . ?
O4 Mo4 O16 156.7(3) . . ?
O14 Mo4 O16 87.1(2) . . ?
O15 Mo4 O16 79.8(2) . . ?
O13 Mo4 O19 164.5(3) . . ?
O4 Mo4 O19 87.1(2) . . ?
O14 Mo4 O19 84.3(2) . . ?
O15 Mo4 O19 70.9(2) . . ?
O16 Mo4 O19 70.6(2) . . ?
O17 Mo6 O31 102.8(3) . . ?
O17 Mo6 O15 102.0(3) . . ?
O31 Mo6 O15 94.0(3) . . ?
O17 Mo6 O11 97.8(3) . . ?
O31 Mo6 O11 157.6(2) . . ?
O15 Mo6 O11 90.3(3) . . ?
O17 Mo6 O29 99.2(3) . . ?
O31 Mo6 O29 87.2(3) . . ?
O15 Mo6 O29 158.0(2) . . ?
O11 Mo6 O29 80.8(2) . . ?
O17 Mo6 O19 177.2(2) . . ?
O31 Mo6 O19 77.1(2) . . ?
O15 Mo6 O19 75.3(2) . . ?
O11 Mo6 O19 82.8(2) . . ?
O29 Mo6 O19 83.6(2) . . ?
O7 Mo2 O2 103.7(3) . . ?
O7 Mo2 O11 100.9(3) . . ?
O2 Mo2 O11 100.3(3) . . ?
O7 Mo2 O6 98.6(3) . . ?
O2 Mo2 O6 93.8(3) . . ?
O11 Mo2 O6 152.3(3) . . ?
O7 Mo2 O21 90.6(3) . . ?
O2 Mo2 O21 165.2(3) . . ?
O11 Mo2 O21 80.1(2) . . ?
O6 Mo2 O21 80.2(2) . . ?
O7 Mo2 O9 167.9(3) . . ?
O2 Mo2 O9 85.2(2) . . ?
O11 Mo2 O9 85.1(2) . . ?
O6 Mo2 O9 72.4(2) . . ?
O21 Mo2 O9 80.1(2) . . ?
O37 Mo9 O21 105.4(3) . . ?
O37 Mo9 O29 104.9(3) . . ?
O21 Mo9 O29 93.1(3) . . ?
O37 Mo9 O25 99.0(3) . . ?
O21 Mo9 O25 92.0(3) . . ?
O29 Mo9 O25 153.3(3) . . ?
O37 Mo9 O36 97.5(3) . . ?
O21 Mo9 O36 156.7(3) . . ?
O29 Mo9 O36 85.1(3) . . ?
O25 Mo9 O36 80.0(2) . . ?
O37 Mo9 O27 166.9(2) . . ?
O21 Mo9 O27 84.6(2) . . ?
O29 Mo9 O27 82.6(2) . . ?
O25 Mo9 O27 71.8(2) . . ?
O36 Mo9 O27 72.1(2) . . ?
O22 Mo5 O8 102.4(3) . . ?
O22 Mo5 O26 101.2(3) . . ?
O8 Mo5 O26 89.6(3) . . ?
O22 Mo5 O10 99.7(3) . . ?
O8 Mo5 O10 94.7(3) . . ?
O26 Mo5 O10 157.2(3) . . ?
O22 Mo5 O28 100.0(3) . . ?
O8 Mo5 O28 157.5(2) . . ?
O26 Mo5 O28 83.9(3) . . ?
O10 Mo5 O28 83.7(3) . . ?
O22 Mo5 O20 171.3(3) . . ?
O8 Mo5 O20 83.8(2) . . ?
O26 Mo5 O20 84.8(2) . . ?
O10 Mo5 O20 73.4(2) . . ?
O28 Mo5 O20 74.3(2) . . ?
O33 Mo8 O28 102.9(3) . . ?
O33 Mo8 O18 102.5(3) . . ?
O28 Mo8 O18 92.6(3) . . ?
O33 Mo8 O35 100.5(3) . . ?
O28 Mo8 O35 93.4(3) . . ?
O18 Mo8 O35 154.3(3) . . ?
O33 Mo8 O30 99.5(3) . . ?
O28 Mo8 O30 157.5(3) . . ?
O18 Mo8 O30 83.6(3) . . ?
O35 Mo8 O30 81.4(3) . . ?
O33 Mo8 O20 174.9(3) . . ?
O28 Mo8 O20 74.9(2) . . ?
O18 Mo8 O20 73.2(2) . . ?
O35 Mo8 O20 84.4(2) . . ?
O30 Mo8 O20 82.8(2) . . ?
O24 Mo10 O23 104.0(3) . . ?
O24 Mo10 O25 100.1(3) . . ?
O23 Mo10 O25 95.8(3) . . ?
O24 Mo10 O26 98.6(3) . . ?
O23 Mo10 O26 88.7(3) . . ?
O25 Mo10 O26 159.1(3) . . ?
O24 Mo10 O38 99.8(3) . . ?
O23 Mo10 O38 155.9(2) . . ?
O25 Mo10 O38 84.0(3) . . ?
O26 Mo10 O38 83.6(2) . . ?
O24 Mo10 O27 170.5(2) . . ?
O23 Mo10 O27 84.5(2) . . ?
O25 Mo10 O27 74.4(2) . . ?
O26 Mo10 O27 85.8(2) . . ?
O38 Mo10 O27 72.2(2) . . ?
O39 Mo11 O36 102.6(3) . . ?
O39 Mo11 O38 102.6(3) . . ?
O36 Mo11 O38 93.6(3) . . ?
O39 Mo11 O34 101.6(3) . . ?
O36 Mo11 O34 90.4(3) . . ?
O38 Mo11 O34 154.0(3) . . ?
O39 Mo11 O35 97.9(3) . . ?
O36 Mo11 O35 159.0(2) . . ?
O38 Mo11 O35 86.0(3) . . ?
O34 Mo11 O35 81.3(3) . . ?
O39 Mo11 O27 175.8(3) . . ?
O36 Mo11 O27 75.8(2) . . ?
O38 Mo11 O27 73.8(2) . . ?
O34 Mo11 O27 82.3(2) . . ?
O35 Mo11 O27 84.0(2) . . ?
O12 Mo3 O3 105.2(3) . . ?
O12 Mo3 O10 101.5(3) . . ?
O3 Mo3 O10 94.0(3) . . ?
O12 Mo3 O14 100.7(3) . . ?
O3 Mo3 O14 91.1(3) . . ?
O10 Mo3 O14 155.0(3) . . ?
O12 Mo3 O18 96.5(3) . . ?
O3 Mo3 O18 158.2(3) . . ?
O10 Mo3 O18 83.2(2) . . ?
O14 Mo3 O18 83.0(2) . . ?
O12 Mo3 O20 167.1(3) . . ?
O3 Mo3 O20 86.7(2) . . ?
O10 Mo3 O20 72.2(2) . . ?
O14 Mo3 O20 83.7(2) . . ?
O18 Mo3 O20 71.8(2) . . ?
O4S N6T O9S 173(3) . . ?
Mo1 O1 La1 136.2(3) . . ?
Mo2 O2 La1 136.9(3) . . ?
Mo3 O3 La1 161.3(3) . . ?
Mo4 O4 La1 154.2(3) . . ?
Mo1 O6 Mo2 121.4(3) . . ?
Mo5 O8 Mo1 156.0(3) . . ?
P1 O9 Mo2 128.8(3) . . ?
P1 O9 Mo1 129.4(3) . . ?
Mo2 O9 Mo1 89.58(19) . . ?
Mo5 O10 Mo3 124.8(3) . . ?
Mo2 O11 Mo6 158.0(3) . . ?
Mo4 O14 Mo3 141.3(3) . . ?
Mo6 O15 Mo4 123.3(3) . . ?
Mo7 O16 Mo4 125.6(3) . . ?
Mo8 O18 Mo3 125.1(3) . . ?
P1 O19 Mo6 126.7(3) . . ?
P1 O19 Mo4 124.5(3) . . ?
Mo6 O19 Mo4 90.41(19) . . ?
P1 O19 Mo7 125.0(3) . . ?
Mo6 O19 Mo7 88.89(18) . . ?
Mo4 O19 Mo7 90.10(19) . . ?
P1 O20 Mo5 125.1(3) . . ?
P1 O20 Mo3 125.5(3) . . ?
Mo5 O20 Mo3 89.21(18) . . ?
P1 O20 Mo8 128.1(3) . . ?
Mo5 O20 Mo8 87.40(18) . . ?
Mo3 O20 Mo8 89.18(19) . . ?
Mo9 O21 Mo2 146.0(3) . . ?
Mo10 O23 Mo1 154.4(3) . . ?
Mo10 O25 Mo9 123.1(3) . . ?
Mo5 O26 Mo10 143.4(3) . . ?
P1 O27 Mo10 124.2(3) . . ?
P1 O27 Mo11 128.9(3) . . ?
Mo10 O27 Mo11 90.08(19) . . ?
P1 O27 Mo9 123.6(3) . . ?
Mo10 O27 Mo9 89.6(2) . . ?
Mo11 O27 Mo9 88.88(18) . . ?
Mo8 O28 Mo5 123.3(3) . . ?
Mo9 O29 Mo6 150.0(3) . . ?
Mo7 O30 Mo8 148.2(4) . . ?
Mo6 O31 Mo7 122.1(3) . . ?
Mo7 O34 Mo11 151.6(3) . . ?
Mo8 O35 Mo11 155.5(3) . . ?
Mo11 O36 Mo9 123.2(3) . . ?
Mo11 O38 Mo10 122.9(3) . . ?
N6S O9S N6T 162(2) . . ?
O9 P1 O20 111.0(3) . . ?
O9 P1 O19 110.8(3) . . ?
O20 P1 O19 108.0(3) . . ?
O9 P1 O27 109.8(3) . . ?
O20 P1 O27 108.3(3) . . ?
O19 P1 O27 108.9(3) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 O4 2.451(6) . ?
La1 O4 2.451(6) 2 ?
La1 O3 2.474(6) 2 ?
La1 O3 2.474(6) . ?
La1 O2 2.489(6) . ?
La1 O2 2.489(6) 2 ?
La1 O1 2.501(6) . ?
La1 O1 2.501(6) 2 ?
Mo7 O32 1.697(6) . ?
Mo7 O30 1.813(6) . ?
Mo7 O16 1.860(6) . ?
Mo7 O34 1.902(6) . ?
Mo7 O31 2.065(6) . ?
Mo7 O19 2.477(6) . ?
Mo1 O5 1.693(6) . ?
Mo1 O1 1.751(6) . ?
Mo1 O6 1.871(6) . ?
Mo1 O8 1.987(6) . ?
Mo1 O23 2.099(6) . ?
Mo1 O9 2.376(5) . ?
Mo4 O13 1.694(6) . ?
Mo4 O4 1.744(6) . ?
Mo4 O14 1.859(6) . ?
Mo4 O15 2.050(6) . ?
Mo4 O16 2.054(6) . ?
Mo4 O19 2.444(6) . ?
Mo6 O17 1.698(6) . ?
Mo6 O31 1.829(6) . ?
Mo6 O15 1.850(6) . ?
Mo6 O11 1.986(6) . ?
Mo6 O29 1.992(6) . ?
Mo6 O19 2.392(6) . ?
Mo2 O7 1.704(6) . ?
Mo2 O2 1.743(6) . ?
Mo2 O11 1.873(6) . ?
Mo2 O6 1.958(6) . ?
Mo2 O21 2.171(6) . ?
Mo2 O9 2.365(6) . ?
Mo9 O37 1.701(6) . ?
Mo9 O21 1.784(6) . ?
Mo9 O29 1.842(6) . ?
Mo9 O25 1.968(6) . ?
Mo9 O36 2.045(6) . ?
Mo9 O27 2.448(6) . ?
Mo5 O22 1.684(6) . ?
Mo5 O8 1.825(6) . ?
Mo5 O26 1.897(6) . ?
Mo5 O10 1.905(6) . ?
Mo5 O28 2.020(6) . ?
Mo5 O20 2.415(5) . ?
Mo8 O33 1.690(6) . ?
Mo8 O28 1.842(6) . ?
Mo8 O18 1.862(6) . ?
Mo8 O35 1.892(6) . ?
Mo8 O30 2.048(6) . ?
Mo8 O20 2.506(6) . ?
Mo10 O24 1.692(6) . ?
Mo10 O23 1.791(6) . ?
Mo10 O25 1.905(6) . ?
Mo10 O26 1.958(6) . ?
Mo10 O38 2.024(6) . ?
Mo10 O27 2.383(6) . ?
Mo11 O39 1.698(6) . ?
Mo11 O36 1.838(6) . ?
Mo11 O38 1.854(6) . ?
Mo11 O34 1.930(6) . ?
Mo11 O35 1.996(6) . ?
Mo11 O27 2.432(6) . ?
Mo3 O12 1.693(6) . ?
Mo3 O3 1.728(6) . ?
Mo3 O10 1.943(6) . ?
Mo3 O14 1.965(6) . ?
Mo3 O18 2.050(6) . ?
Mo3 O20 2.442(6) . ?
N6S O9S 1.11(5) . ?
N6T O4S 1.17(4) . ?
N6T O9S 1.61(4) . ?
O9 P1 1.529(6) . ?
O19 P1 1.540(6) . ?
O20 P1 1.539(6) . ?
O27 P1 1.548(6) . ?
